Viswanathan S Saji and Han Cheol Choe20499⋅95%; Aldrich, USA), copper nitrate (Cu(NO3)2⋅3H2O,99%; Junsei, Japan) and titanium butoxide (Ti(O(CH2)3CH3)4; 97%, Sigma-Aldrich, USA). The precursor chemi-cals were weighed and mixed in the molar ratio ofCa : Cu : Ti = 1 : 3 : 4. The solvent used was 2-methoxyethanol (C3H8O2, 99⋅9%, Sigma-Aldrich, USA). Theselection of the precursor chemicals was done with aview to favour maximum chelating effect. The total vol-ume of the reagents to the solvent was kept in a ratio of1 : 2. The mixed solution was subjected to stirring using amagnetic stirrer for 10 h. Spin coating was carried out at3000 rpm for 20 s. The substrate used was commerciallyavailable heavily boron-doped silicon. The coated filmwas subjected to pyrolysis at a temperature of 500°C for2 min in air. The heating rate used from room tempera-ture to the pyrolysis temperature was ~ 50°C/s (time ofheating, 10 s). The procedure of coating and pyrolysiswas repeated two to three times in order to obtain adesired film thickness of ~ 500 nm. Lastly the film wassubjected to sintering at different temperatures rangingfrom 700–800°C for 8 min in air. A heating rate of~ 75°C/min was used from the pyrolysis temperature tothe sintering temperature (time of heating from 500–800°C, 4 min). The final pyrolysis and sintering wereperformed in a single step. Rapid thermal annealing(RTA, ULVAC-RIKO, MILA-3000) was employed. Thecooling rate was ~25°C/min. Selection of the pyrolysis andsintering temperature was in accordance with the TG/DTA studies of the dried precursor solution (not shownhere). Selection of optimized temperature, time and heat-ing rate for both pyrolysis and sintering was essential forgetting pure phase CCTO. Figure 1 shows a flow chart ofthe film processing.2.2 Phase and microstructureThe crystalline structure of sintered films was examinedusing X-ray diffraction (XRD, X’pert Pro, Philips) usingCuKα radiation. Scanning electron microscope was usedto study the film surface morphology as well as for filmthickness measurements (FE–SEM, Hitachi 4800). BeforeSEM observation, thin gold film was deposited on thesample surface.2.3 Dielectric propertiesAn impedance analyzer (HP 4194A, Hewlett-Packard)was used to measure the capacitance and dielectric loss ofthe film in the frequency range 1 kHz–1 MHz at roomtemperature, 25 ± 1°C. Dielectric constant was calculatedfrom the obtained capacitance values and the film thick-ness. Top platinum electrodes with an area of 5 × 10–8m2were deposited by d.c. magnetron sputtering on the filmsurface using a shadow mask for the dielectric measure-ments. The time of platinum sputtering was 20 min.3. Results and discussion3.1 Phase and microstructureFigure 2 represents the XRD patterns recorded for theCCTO films as a function of sintering temperature. At thetemperature range of 600–700°C, CuO was the mainconstituent of the crystallized phase. Along with the CuOphase, anatase and rutile forms of TiO2 were detected.The unidentified peaks may correspond to titanium orFigure 1. Flow chart for CCTO thin film processing.Figure 2. XRD pattern recorded as a function of sinteringtemperature. The substrate peak was removed for clarity.
Chemical solution deposition of CaCu3Ti4O12 thin film 205Figure 3. SEM images of CCTO thin films as a function of sintering temperature.silicon based compounds. However, when the sinteringtemperature was increased to 750°C, the second phasesdisappeared and pure phase CCTO thin film wasobtained. The film exhibited (220) preferential orientation.The diffraction patterns showed distinct (220), (400),(422) and (440) peaks along with low intensity peaks.The peaks match with the corresponding peaks in bulkCCTO, revealing polycrystalline nature of the film withcubic perovskite structure (space group, Im3) (Bochuet al 1979). With further increase in sintering temperatureand sintering time, no major structural changes wereobserved.Representative SEM surface and lateral imagesobtained for the CCTO films as a function of sinteringtemperature is shown in figure 3. The SEM images sup-port the XRD results revealing polycrystalline nature.The film exhibited exaggerated grain growth and duplexmicrostructure consisting of large grains in excess of400 nm in length and small grains of < 200 nm. Theexaggerated grain growth may be attributed to the CuObased liquid phase sintering (Leret et al 2007). Trappedpores were observed in large grains and in grain bounda-ries when the sintering temperature was above 900°C.The pores may have developed from the abnormal graingrowth and the grain boundaries moving quickly duringthe sintering process (Liu et al 2007). Due to the exa-ggerated grain growth, any significant variation in graingrowth with sintering temperature was not observed. Lat-eral view image in the figure corresponds to a three-timespin coated film sintered at 800°C. The image indicates awell densified structure with some columnar grains. Theaverage thickness of a three-time spin coated film was~ 400 nm. The interface between the CCTO film andbottom electrode was sharp implying negligible inter-diffusion across the interface.3.2 Dielectric propertiesThe variation of k and the dielectric loss recorded for thefilms as a function of frequency of measurement is shownin figure 4. The dielectric measurements were carried outin four selected frequencies, viz. 1 kHz, 100 kHz,500 kHz and 1 MHz. The CCTO film sintered at 750°Cshowed a k value of ~ 2100 and a loss tangent of ~ 0⋅06 at1 kHz. The decrease in k when sintering temperature wasabove 900°C is associated with the trapped porosity asobserved by SEM. At higher measuring frequencies, kdecreased gradually, accompanied by a correspondingincrease in loss factor.The large k at lower frequencies is suggested to beassociated with the Maxwell-Wagner contributions of
Viswanathan S Saji and Han Cheol Choe206Figure 4. Dielectric constant and dielectric loss of CCTO thin film at different sintering temperaturesas a function of measuring frequency.depletion layers at grain boundaries or interfaces betweenthe sample and contacts (Adams et al 2002; Lukenheimeret al 2004). So far, the internal barrier layer capacitor(IBLC) model has been widely accepted as the mostlikely mechanism to elucidate the CDC in CCTO. Thedifference of conductivity between grain boundary andgrain volume causes the charge accumulation on the grainboundary on a mesoscopic scale, which results in largequantity boundary barrier layer capacitors. On a macro-scopic scale, the electrode contact effect may play asignificant role in CDC. Liu et al (2008) showed thatelectrode and grain boundary act as two depletion layerswith distinct relaxation. On increasing the frequency, thespace charge polarization relaxes leading to decrease in k.It has been shown that the frequency of dielectric relaxa-tion was much lower in the case of CCTO film whencompared to that of the bulk ceramic (Shri Prakash et al2008). The dielectric properties of the film obtained inthe present work is comparable with that reported forpolycrystalline CCTO thin films (Si et al 2002; Fang andShen 2003; Fang et al 2004; Shri Prakash et al 2008).The high dielectric constant obtained for the CCTO filmin the present study indicates its possible application inmicroelectronic devices.4. ConclusionsHighly oriented CCTO thin films were successfullydeposited on boron doped silica substrate at a sinteringtemperature of 750°C. Effect of sintering temperature onthe phase and microstructure of the film was investigated.The film formed was polycrystalline in nature with (220)preferential orientation. SEM microstructures of the filmsrevealed a bimodal size distribution of grains. Dielectricconstant and loss tangent at 1 kHz obtained for the filmsintered at 750°C was k ~ 2000 and tanδ ~ 0⋅05, respec-tively.AcknowledgementThe authors express their sincere gratitude to ProfessorYong Soo Cho, Department of Materials Science andEngineering, Yonsei University, Korea.
Chemical solution deposition of CaCu3Ti4O12 thin film 207ReferencesAdams T B, Sinclair D C and West A R 2002 Adv. Mater. 141321Adams T B, Sinclair D C and West A R 2006 Phys. Rev. B73094124Bochu B, Deschizeaux M N and Joubert J C 1979 J. Solid StateChem. 29 291Briźe V, Gruener G, Wolfman J, Fstyeyeva K, Tabellout M andGervais F 2006 Mater. Sci. Eng. B129 135Chung S Y, Kim I L and Kang S J L 2004 Nat. Mater. 3 774Cohen M H, Neaton J B, He L and Vanderbilt D 2003 J. Appl.Phys. 94 3299Fang L and Shen M 2003 Thin Solid Films 440 60Fang L, Shen M and Cao W 2004 J. Appl. Phys. 95 6483Feng L, Wang Y, Yan Y, Cao G and Jiao Z 2006 Appl. Surf.Sci. 253 2268Homes C C, Vogt T, Shapiro S M, Wakimoto S and RamirezA P 2001 Science 293 673Jiménez R, Calzada M L, Bretos I, Goes J C and Sombra A S B2007 J. Eur. Ceram. Soc. 27 3829Leret P, Fernandez J F, de Frutos J and Fernandez-Hevia D2007 J. Eur. Ceram. Soc. 27 3901Liu L, Fan H, Fang P and Jin L 2007 Solid State Commun. 142573Liu L, Fan H, Wang L, Chen X and Fang P 2008 Philos. Mag.88 537Lu W, Feng L, Cao G and Jiao Z 2004 J. Mater. Sci. 39 3523Lukenheimer P, Fichtl R, Ebbinghaus S G and Loidl A 2004Phys. Rev. B70 172102.Martin L, Guillemet-Fritsch S, Durand B, Levchenko A A,Navrotsky A and Lebey T 2008 J. Am. Ceram. Soc. 91 485Ramirez A P, Subramanian M A, Gardel M G, Blumberg G, LiD, Vogt T and Shapiro S M 2000 Solid State Commun. 115 217Schwartz R W 1997 Chem. Mater. 9 2325Shri Prakash B, Varma K B R, Michau D and Maglione M 2008Thin Solid Films 516 2874Si W, Cruz E M, Johnson P D, Barnes P W, Woodward P andRamirez A P 2002 Appl. Phys. Lett. 81 2056Subramanian M A, Li D, Duan N, Reisner B A and Sleight A W2000 J. Solid State Chem. 151 323Sun D L, Wu A Y and Yin S T 2008 J. Am. Ceram. Soc. 91 169